- Email: [email protected]

Physica E 15 (2002) 238 – 242 www.elsevier.com/locate/physe

Carrier self-energy and photoluminescence spectrum in quantum Hall system Ming-Che Changa;∗ , H.H. Chengb a Department

of Physics, National Taiwan Normal University, 88 Sec 4 Ting-Chou Rd, Taipei, 116, Taiwan for Condensed Matter Sciences, National Taiwan University, Taipei, 116, Taiwan

b Center

Received 5 May 2002; received in revised form 8 August 2002; accepted 6 September 2002

Abstract In this paper, we study electronic screening and its subsequent in0uence on the electron self-energy in quantum Hall system. We focus on two issues: how the width of quantum well and the strength of disorder a3ect the electron self-energy. It is found that a wider quantum well has a smaller self-energy correction, and a stronger disorder yields a smaller self-energy oscillation with respect to the magnetic 4eld. We have also compared the theoretical many-body energy spectra with actual photoluminescence spectra of a modulation-doped quantum well in a strong magnetic 4eld. ? 2002 Elsevier Science B.V. All rights reserved. PACS: 73:40.Hm; 78:66.−w Keywords: Quantum Hall e3ect; Photoluminescence

Calculation of electron self-energy in quantum Hall system is crucial in understanding phenomena such as exchange-enhanced Zeeman splitting [1], the blue shift of photoluminescence (PL) spectrum near integer 4lling factors [2,3], the energy spectrum in modulated systems [4], and hysteresis e3ect [5,6]. The simplest many-body correction is calculated using the Hartree– Fock approximation (HFA). This is not necessarily a good approximation but often is chosen for its simplicity. In some cases, screened HFA is used [1,4], but in the absence of justi4cation this may not necessarily yield an improved result over the HFA. In fact, it is known that, in the 4eld-free case [7], screened ∗

Corresponding author. Tel.: +886229317515; +886229326408. E-mail address: [email protected] (Ming-Che Chang).

fax:

HFA yields a worse result. Also, in the calculation of the PL spectrum for a quantum Hall system, using the screened HFA would predict a red shift, instead of the observed blue shift, near integer 4lling factors. In this paper, we calculate the electron self-energy beyond the screened HFA by including the Coulombhole term. We study in detail the change of self-energy as various physical parameters, such as the width of quantum well and the strength of disorder, are changed [8]. 1 Calculating the conduction electron energy together with the valence hole energy enables us to calculate the PL spectra since the latter are largely determined by the energy di3erence between electrons and holes. The outline of this calculation has been published in the study of PL in Refs. [2,3]. It is believed 1

This paper studies how the distance between the electron layer and the hole layer a3ects the PL spectrum.

1386-9477/02/$ - see front matter ? 2002 Elsevier Science B.V. All rights reserved. PII: S 1 3 8 6 - 9 4 7 7 ( 0 2 ) 0 0 6 6 0 - 4

Ming-Che Chang, H.H. Cheng / Physica E 15 (2002) 238 – 242

that their calculations are applicable to dirtier samples where disorder e3ect is dominant, and many-body interactions are added later on as perturbations. On the contrary, for high mobility samples where many-body e3ects are dominant, various di3erent spectral features might appear. For example, the abrupt red shift near 4lling factor = 1 has been attributed to di3erent recombination mechanisms at = 1+ and 1− [9–11]. In the vicinity of = 1 quantum Hall ferromagnet, it costs less energy to create a skyrmion than to create a quasi-particle. Therefore, skyrmion-related features of the PL spectrum may appear [12–14]. Some groups observed a low-energy satellite peak in PL as ¿ 2, which has been explained as a signature of Anderson-Fano-like resonance [9,11,15]. In other occasions, multiplet structure near the neutral exciton recombination line has been observed, which is due to either charged excitons or low-lying many-body excitations [16,17]. The motivation of this work is to explain the PL spectra reported in Ref. [18], in which none of these many-body features seem to be relevant. The observed blue shift near integer 4lling factors is best explained using Katayama’s and Uenoyama’s slightly di3erent theories [2,3]. Katayama and Ando use the plasmon-pole approximation, while Uenoyama and Sham use the quasi-static approximation, to obtain the dielectric function. We will follow the latter approach, which is computationally less involved, but is expected to be less accurate at high magnetic 4elds [19]. In the quasi-static random phase approximation, the electron energy is composed of the bare particle energy, the screened exchange energy and the Coulomb-hole energy [20–23]: 2 En = En0 + nsx + nch ;

(1)

where En0 = (n + 1=2)˝!c + ge e B, n is the Landau level (LL) index, ge and e are the e3ective g-factor and the magnetic moment of electrons, respectively. For the many-body corrections, we have [3] d2 q ˜ nsx = − V nn (q)n ; (2)2 n

2

See Appendix B of Ref. [23] for a very nice derivation.

nch =

1 2 n

239

d2 q ˜ [V nn (q) − Vnn (q)]; (2)2

(2)

where q is the magnitude of the momentum q, Vnn (q) = F ⊥ (q)Fnn (q)V (q), F ⊥ (q) is the form factor of the electron envelope function along the z-direction, Fnn (q) is the form factor associated with the Landau orbitals in the x–y plane, and n is the electron 4lling factor in the nth LL. The tilde indicates that the Coulomb potential V (q) = 2e2 =0 q is screened, V˜ (q) = V (q)=(q), where (q) is the static dielectric function to be explained in more details below. The form factors are determined by F ⊥ (q) = dz d z |(z)|2 |(z )|2 e−q|z−z | ;

Fnn (q) = |n|eiq· |n |2

= (n !=n!)(q2l2B =2)n−n e−q

2 2 lB =2

2 2 2 [Ln−n n (q lB =2)]

(for n ¿ n );

(3)

where (z) is the electron envelope function along the z-direction, is the cyclotron coordinate, lB = ˝=eB is the magnetic length, and L are the associated Laguerre polynomials. Notice that in the self-energy corrections above, the screened exchange part is a function of the carrier population. Therefore, for a system with dilute carriers, such an energy correction can be neglected because there is almost no quantum exchange e3ect. This is the case when these formulas are used to calculate the self-energy of dilute photo-excited valence holes in the PL experiment. Because of the low hole density, the self-energy for holes are dominated by the Coulomb-hole term only. The dielectric function describes the e3ectiveness of screening and it is sensitive to the location of the Fermi level. The discrete nature of the LLs leads to prominent variation of this quantity as the magnetic 4eld is changed. It can be separated to a dominant part related to intra-LL transitions and a minor part related to inter-LL transitions [3], (q) = 1 + F ⊥ (q)V (q)[D(EF ) − inter (q)]:

(4)

The former is proportional to the disorder-broadened density of states (per unit area) D(E), which is assumed to be a Gaussian (for each LL) with a width .

Ming-Che Chang, H.H. Cheng / Physica E 15 (2002) 238 – 242

That is, D(E) =

n

s 2l2B

0 2

2 e−2(E−En =) ;

Σsx

(5)

where s (=1 in our case) is the spin degeneracy. The√width depends on the magnetic 4eld, = (= B)˝!c , in which B is in units of Tesla and depends on sample quality and is of the order unity. The inter-LL part inter (q) is given as s n − n |n|eiq· |n |2 : (6) inter (q) = 2l2B nn En0 − En0 It becomes more important in a weak magnetic 4eld due to the smaller LL separations. In addition, its presence is also required for the dielectric function to satisfy the f-sum rule [3]. Combining this dielectric function with the formulas (1)–(3) above, we have calculated the electron self-energy for a n-type modulation-doped InGaAs/GaAs QW. The QW is approximated as a square well with a height V0 and a width d. The electron envelope function is approximated as a Gaussian 2 −"z 2 . It is then conwith a width ", |(z)| = "=e venient to obtain an analyticform for the form factor √ 2 F ⊥ (q) = (2= )eq =2" erfc( q2 =2"). The width " is determined by minimizing the electron energy in the Hatree approximation [24]. For a QW with a height P [18], the optiV0 = 57 meV and a width d = 200 A P 2. mized parameter for the Gaussian is "=2:0×10−3 = A For the InGaAs/GaAs QW sample being used in the PL experiment [18], the electron e3ective mass is 0:0622 me , ge = −2; 0 = 12, and the electron density after optical pumping is 2:7 × 1011 =cm2 . The parameter in the LL broadening is chosen as 1=2, which gives = 4:68 meV at B = 10 T. For comparison, the cyclotron energy is 18:6 meV at 10 T. It is known that the electron cyclotron energy ˝!c is proportional to B and typical√electron interaction energy e2 =0 lB is proportional to B. For reference, these two energies become equal at B = 6:32 T. In Fig. 1, we plot the screened exchange energies and the Coulomb-hole energies for electrons in the lowest three LLs. The 4lling factors are 1–3 when the magnetic 4elds are 11.12, 5.56, and 3:73 T, respectively. When B ¿ 11:12 T, the electrons are populated in the LLL so only 0sx and 0ch are of interest. As the magnetic 4eld gets smaller, electrons are populated in more than one LL and several self-energies

electron self-energy (meV)

240

-2

-4

Σch

-6

-8 0

5

10 15 magnetic field (T)

20

Fig. 1. Screened exchange energies and Coulomb-hole energies for the lowest three LLs are shown ( = 1=4). The curves with downward cusps are nsx ; the curves with upward cusps are nch . Solid lines, dotted lines, and dashed lines are for n = 0; 1, and 2, respectively. The bold solid line below is the total self-energy for the LLL, which is the sum of the two solid lines above.

for di3erent LLs are plotted. It can be seen that the Coulomb-hole energies for di3erent LLs have roughly the same values, which makes the curves diQcult to be distinguished in weak magnetic 4elds. At integer 4lling factors, the electron gas is insulator-like and the screening is less e3ective. Therefore, there is a larger (in magnitude) negative screened exchange energy. This leads to the downward cusps in the 4gure. The Coulomb-hole energy is the energy reduction due to the charge de4ciency around a charged carrier. At integer 4lling factors, the electrons are “locked” at their respective Landau orbitals, which means that it is more diQcult to distort the wave function and create a Coulomb hole. Therefore, the negative Coulomb-hole energy is smaller (in magnitude) at integer 4lling factors. This gives the upward cusps in the 4gure. For electrons, the total self-energy, which is the sum of the two terms above, is less-sensitive to the 4lling factor because this two opposite trends from the screened exchange energy and the Coulomb-hole energy cancel each other [2,3]. (see the bold line in Fig. 1). Naively, we expect the magnitudes of the cusps √ at integer 4lling factors to be proportional to B, because the electron–electron interaction, which

Ming-Che Chang, H.H. Cheng / Physica E 15 (2002) 238 – 242

0

241

-8

-2 -9 -4

energy (meV)

electron self-energy (meV)

Σsx

Σch

-10

-6

-8

0

5

10 15 magnetic field (T)

20

-11 0

5

10

15

magnetic field (T)

Fig. 2. Screened exchange energy and Coulomb-hole energy for electrons in the LLL. Solid lines are for a QW with width P dotted lines are for a QW with a width d = 300 A. P The d = 200 A; impurity broadening parameter is 1/4 for both cases. Dot-dashed P and = 1=2. lines are for d = 200 A

Fig. 3. Crosses are the PL energies for electrons transiting from the lowest electron LL to the highest valence hole LL that is permitted by the selection rule. The part linearly increasing with B has been removed, as explained in the text. The solid line is the theoretical result ( = 1=2).

gives rise to the screened exchange term √ and the Coulomb-hole term, is proportional to B. However, the e3ective interactions in di3erent LLs can be very di3erent because of the Landau-orbital form ⊥ factors Fnn , which reduce rapidly as n gets √ larger. This is why the cusps diminish faster than B as B is decreased. It is expected that, because the e3ective twodimensional Coulomb interaction is reduced in a wider QW, the self-energy will be smaller. It is interesting to know quantitatively the connection between the width of the QW and the self-energy correction. In Fig. 2, we show the self-energy for the electrons in the LLL in a wider QW (dotted lines). It can be seen that the energies at the cusps remain largely unchanged, but the energies at half-integer 4llings are indeed reduced by several meVs. We have also investigated the e3ect of impurity broadening on the self-energy. In general, thinner disorder-broadened LLs would give larger self-energy oscillations. In Fig. 2, we see that as the parameter is varied (dot-dashed lines), the cusp energies also remain largely unchanged. But the energy shifts at half-integer 4llings are signi4cant. Unlike the changes due to 4nite QW width that have both 0sx

and 0ch shift up. The shifts due to impurity broadening are opposite for 0sx and 0ch . Therefore, it would give a very minor change to the total self-energy. Even though we only show the result for the LLL in Fig. 2, the behavior for higher LLs are basically the same. In Fig. 3, the theoretical PL energy is compared with the experimental data. The PL energy is the di3erence between the electron energy and PL e h e the hole energy, ENN = EN − EN , where EN is composed of three parts as shown in Eq. (1), ENh is composed of the bare particle energy, to be calculated from the Luttinger formalism [18], and the Coulomb-hole energy. The selection rule requires UN = 1, where N = n + mj − 1=2, in which n is the LL index, and mj is the spin-component in the z-direction. We have calculated the Coulomb-hole energy for holes using the following parameters: hole e3ective mass mh = 0:094me , and the QW at the valence band has a depth V0 = 68 meV and P The solid line in Fig. 3 repa width d = 200 A. sx(e) resents N + Nch(e) − Nch(h) . The crosses are the PL peak energies being measured [18]. To emphasize the oscillating behavior, we have subtracted from the experimental data a part &B that is

242

Ming-Che Chang, H.H. Cheng / Physica E 15 (2002) 238 – 242

linearly proportional to the magnetic 4eld. The slope & (=0:9 meV=T) is the sum of the slopes from the bare-electron energy and from the hole energy calculated using the eight-band Luttinger formalism. The data has also been vertically shifted to 4t the curve. The only essential adjustable parameter in this calculation is the disorder-broadening parameter , which is chosen to be 1=2 for both the electrons and the holes. It can be seen that the magnitudes of the dips between the cusps agree roughly with the experimental data, supporting the aforementioned mechanism for the blue shift. To summarize, we have investigated in details the in0uence of the QW width and the impurity broadening on the self-energy of the electrons in quantum Hall systems. It is found that a wider quantum well has a smaller self-energy correction, and a larger level-broadening yields a smaller self-energy variation with respect to the magnetic 4eld. Comparison with experiment shows that the calculation can explain the observed data reasonably well. These quantitative results might be helpful for experimentalists to 4ne-tune the spectral properties of their samples. M.C.C. thanks M.F. Yang for valuable discussions and the support from Taiwan’s National Science Council via Grant NSC 90-2112-M-003-022. H.H.C. acknowledges the support from the Grant NSC 90-2112-M-002-053.

References [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24]

T. Ando, Y. Uemura, J. Phys. Soc. Jpn. 37 (1974) 1044. S. Katayama, T. Ando, Solid State Commun. 70 (1989) 97. T. Uenoyama, L.J. Sham, Phys. Rev. B 39 (1989) 11044. A. Manolescu, R. Gerhardts, Phys. Rev. B 56 (1997) 9707. A. Manolescu, V. Gudmundsson, Phys. Rev. B 61 (2000) R7858. M.C. Chang, M.F. Yang, Phys. Rev. B 64 (2001) 073302. A.W. Overhauser, Phys. Rev. B 3 (1971) 1888. T. Tsuchiya, S. Katayama, T. Ando, Jpn. J. Appl. Phys. 34 (1995) 4544. P. Hawrylak, M. Potemski, Phys. Rev. B 56 (1997) 12386. N.R. Cooper, D.B. Chklovskii, Phys. Rev. B 55 (1997) 2436. L. Gravier, M. Potemski, P. Hawrylak, B. Etienne, Phys. Rev. Lett. 80 (1998) 3344. T. Portengen, J.R. Chapman, N. Nicopoulos, N.F. Johnson, Phys. Rev. B 55 (1997) R7367. T. Portengen, J.R. Chapman, N. Nicopoulos, N.F. Johnson, Phys. Rev. B 56 (1997) R10052. A.N. Priest, R.J. Nicholas, C. Symons, J.C. Portal, C.T. Foxon, J.J. Harris, Physica B 256 (1998) 347. M.J. Manfra, B.B. Goldberg, L. Pfei3er, K. West, Phys. Rev. B 57 (1998) R9467. S. Glasberg, G. Finkelstein, H. Shtrikman, I. Bar-Joseph, Phys. Rev. B 59 (1999) R10425. F.M. Munteanu, Y. Kim, C.H. Perry, D.G. Rickel, J.A. Simmons, J.L. Reno, Solid State Commun. 111 (1999) 665. H.H. Cheng, M.C. Chang, R.J. Nicholas, C.P. Lee, preprint. G.E.W. Bauer, Phys. Rev. B 45 (1992) 9153. L. Hedin, Phys. Rev. 139 (1965) A796. L. Hedin, J. Phys.: Condens. Matter 11 (1999) R489. H. Haug, S. Schmitt-Rink, Prog. Quant. Electron. 9 (1984) 3. H. Haug, S.W. Koch, Quantum Theory of the Optical and Electronic Properties of Semiconductors, 3rd Edition, World Scienti4c, Singapore, 1994. G.E. Bauer, T. Ando, J. Phys. C 19 (1986) 1537.

Copyright © 2022 COEK.INFO. All rights reserved.